About 4 to 5 tons of molding sand may be required to produce 1 ton of castings.
Poor molding sand ------ poor castings.
Attention to preparing, controlling, handling, and properly using the sand.
Several different types of molding sands are used.
Usually green sand.
GENERAL PROPERTIES OF MOLDING SANDS
Molding sand must be readily moldable and produce defect-free castings.
AFS – sets forth the standard condition of testing the sand properties.
1. GREEN STRENGTH:
Adequate strength and toughness for making and handling the mold.
2. DRY STRENGTH:
Dry sand must have strength to resist erosion and also the metallostatic pressure of the molten metal or else the mold may enlarge.
3. HOT STRENGTH:
Hot molten metal
Metallostatic pressure of the liquid metal bearing against the mold walls may cause mold enlargement, or if the metal is still flowing, erosion, cracks, or breakages may occur unless the sand posses adequate hot strength.
Steam and other gases
The mold must be permeable, i.e. , porous to permit the gases to escape.
5. THERMAL STABILITY:
Heat from the casting causes rapid expansion of the sand surface at the mold-metal interface.
The mold surface may crack, buckle, or flake off (scab ) unless the molding sand is relatively stable dimensionally under rapid heating.
The absence of melting, softening, or adherence of the sand to the casting makes for better casting surface and easier cleaning of the casting.
Ferrous alloys ---- sand with high refractoriness.
The sand should pack well/flow under load.
Sands of low flowability may result in non-uniform hardness.
Soft molds --- enlargement of the casting or roughness of the casting surfaces.
8. PRODUCE GOOD CASTING FINISH:
Finer sands ----- a smoother casting surface.
Heated sands -------- hard and rocklike.
Difficult to remove from the casting
May cause the contracting metal to tear or crack.
10. THE SAND SHOULD BE REUSABLE.
11. EASE OF SAND PREPARATION AND CONTROL.
** Economic production of good casting.
INGREDIENTS OF MOLDING SANDS
Molding sands are actually mixtures of three or more ingredients.
Green sand --- clay, water, sand (SiO 2 ).
Also a number of other ingredients/materials are added.
Silica sand forms 50 to 95 % of the total material in a molding sand.
These sand particles may differ in the following ways:
Average grain size, grain size distribution and grain shape.
Refractoriness and thermal stability.
Generally the purest silica sand, 99.8+ percent SiO 2 is considered the most refractory and thermally stable.
Excessive amounts of iron oxide, alkali oxides and lime can cause objectionable lowering of the fusion point in some sands.
The shape of sand grains may be rounded, angular, or sub-angular depending on their geologic history.
Compounded grains are agglomerated particles of angular or sub-angular sands.
new molding sand
addition of new silica sand
2 to 50 percent
With a suitable water content, it is the principal source of the strength and plasticity of the molding sand.
Natural molding sand ------- sand + clay in minerals
Synthetic molding sands
“ Essentially aggregates of extremely minute crystalline, usually flake-shaped particles that can be classified on the basis of their structure and composition into a few groups which are known as clay minerals.
Single clay minerals
Mixtures of clay minerals
Clay minerals : bentonites, fire clays (kaolinites) and
special clays (halloysite, illite)
1.5 to 8 percent
Activate the clay ----------- develop plasticity and strength.
Water in molding sand is often referred as “tempering” water.
Water in excess -------- free water
The rigid clay coatings of the sand grains may be forced together ---------- develop strength.
Free water ----- lubricant --- makes the sand more plastic and more moldable though the strength may be lowered.
Control of water in sand (clay) is very important.
*finely ground corn flour or
*gelatinized and ground starch from corn.
*0.25 to 2.00 percent
*Increase green or dry strength and collapsibility.
*by-product of coke making.
*up to 2.0 percent
*improve hot strength and casting finish
on ferrous castings
*2 to 8 percent.
*A finally ground soft coal.
* Grey and malleable iron molding sands.
* Improve the surface finish.
*Improve ease of cleaning the castings.
*About 0.4 to 0.8 percent.
* Improve casting finish
*A little fuel oil is sometimes used as a replacement for a small percentage of water, thus lowering the total percentage of moisture present .
*0.5 to 2.0 percent
*Enhance thermal stability.
*Control the expansion of sand by burning out at elevated temperature
* Pulverized silica, finer than 200 mesh, is called silica flour.
*Up to 35 percent
*Increase hot strength
*0.25 to 1.0 percent
*To obtain added hot strength .
*An aluminum silicate mineral
*0.5 to 1.5 percent
* Better thermal stability of the sand
* Riser insulator
*Cane or blackstrap molasses, unrefined, and containing 60 to 70 percent sugar solids, may be used for increased dry strength.
* Dextrins may also be used for the same purpose
PROPERTIES OF GREEN SANDS
Properties depends on several factors.
i) The sand ingredients.
ii) The methods of preparing the sand for molding.
iii) The method of molding employed in using the sand.
iv) Variables related to the casting such as weight, shape, kind of casting alloy and gating design.
Effect of the ingredients:
* Each of the ingredients can have important effects on the properties.
Principal ingredient ----- Silica Sand Grains
Effects of the Sand Grains:
Casting surface finish, mold permeability, sand strength, refractoriness, and expansion characteristics are all influenced by the sand grain portion of the mixture.
Sand-grain contour of the mold cavity.
Fine grains ------ smooth wall at the metal interface.
Sand grains and permeability:
Coarser sand ---- greater permeability
Finer sand ---- lower permeability
The grain size distribution has a pronounced effect on permeability.
1-, 2-, 3-, 4-, and 5-sieve sands ---- sieve analysis
Narrowest distribution range and minimum of fine materials such as silt or clay present ---- most permeable.
Permeability is also promoted by the rounded type of sand grain.
Sand grains and strength:
Strength ----------- surface area of sand grains available for binding.
Fine sands present more surface area and can develop high strength, but of course more clay is required.
Wide size distributions favor strength, while narrow distributions reduce strength.
Angular sand grains ----- more strength
Sand grains and refractoriness:
High refractoriness ----- sand grains of maximum purity and size.
Impurities which discolor silica lower its fusion point.
Finer grains appear to be more easily fused than coarser ones.
Sand grains and Expansion:
Wide size distribution ------ dense packing of the grains ---
cause expansion problems.
Fine sands also expands more.
Effects of Clay:
** Water is necessary to activate the clay.
Clay and Sand Strength:
For a given clay type and content, there is an optimum water content.
The effects of the clay on dry and hot strengths are quite important.
Too low a dry strength permits washing of the sand by the metal, and dirt in the castings.
Too low or too high a hot strength is also undesirable.
Grey-iron sands ----- 20 to 80 psi dry strength
Hot strength of 50 to 80 psi at 1100 F, with less than 0.030 in. per in. expansion is desired.
Aluminum castings --- only green and dry strength have appreciable importance since castings are poured at low temperatures.
Clay Content and Permeability:
Permeabilities are reduced by fine material in the sand.